Presentation on theme: "The New Test Technology for Evaluating the Anti-cracking Performance of Concrete Runway of the Airport under Construction China Airport Construction Group."— Presentation transcript:
The New Test Technology for Evaluating the Anti-cracking Performance of Concrete Runway of the Airport under Construction China Airport Construction Group Corporation of CAAC LIU YAN
Contents Introduction New method- Dumbbell Method Comparative Study of Three Methods Conclusion Engineering Application 4 4
Introduction This presentation introduces one new test technology for evaluating the anti- cracking performance of concrete runway of the airport under construction. The cracking performance of concrete testing under constraint condition is more close to the condition of concrete at job site. The lack of a standard test for early shrinkage cracking resistance has prompted several methods. Three test method for early shrinkage cracking Slab methodRing methodPrism method
1 、 Slab Method 1 wire mesh or steel bar provide constraint Introduce by Karri in 1985 ACI 544.2R for testing Fiber Reinforced Concrete limitation ： crack is irregular and disorder couldn’t provide quick and accurate evaluation
1 、 Slab Method 2 limitation ： coarse aggregate in concrete falling down after vibration The key test part may be mortar,not concrete Recommended by ICBO and RILEM
2 、 Ring Method Ring method pictureObserve and measure the crack Introduced by Roy Carlson from MIT in limitation ： need long time (several days) to wait the crack appear and its poor sensitivity.
3 、 Prism Method Introduced by Springenschmid from Germany in 1960’s. limitation ： inconvenient to use at job site and instruments require high sensitivity and expensive.
Aim for the new method providing a method to evaluate concrete crack performance with: 1 、 quickly testing 2 、 convenient measurement 3 、 can perform test at job site
New method- Dumbbell Method Dumbbell device Dumbbell method with stress risers is invented.
New method- Dumbbell Method The device is made by steel material, which included the fixed-end and adjustable stress risers in the middle which can induce the crack of the concrete specimen. The ends of the device can provide the constraint which makes concrete crack. This method proves to be more effective for the quick crack testing. Dumbbell device
Mechanism Analysis of dumbbell method Mechanism Analysis Under the induction of stress riser and the constraint of the ends of mold, the crack shape is close to a single line,(the line of A-A’). So the crack observation and measurement is more convenient and faster.
Mechanism Analysis of new test method Mechanical analysis of A point and A’ point
Evaluation Index 1 、 ACW (average crack width within 24h) The only crack are divided into six equal portions by five line segments. Record the crack width at the five crossing of crack and line. The average of the five widths is ACW. 2 、 ICT (Initial crack time) ICT is another important index of concrete cracking performance. The later the concrete crack, the better the anti-cracking performance. microscope
Comparative study of three evaluating methods
Concrete mix proportion There are 3 mix proportions and each will be tested by three methods under the same test condition.The fiber reinforced concrete is designed to compare sensitivity of three test method. Fiber dosage is 0.9kg/m3, 1.2kg/m3, 1.5kg/m3. Tests temperature is maintained at 30 ± 2 ℃, relative humidity is maintained at 50 ± 5%. Material (kg/m 3 ) Slump （ mm ） Slump Flow （ mm ） CementSandGravelWaterFiber / / /460 Concrete mix proportion cubic meter
Test results Dumbbell Slab Ring 1.5kg/m 3 Initial crack time2h:15min2h:30min6d Maximum crack width1.07mm0.64mm0.52mm 1.2kg/m 3 Initial crack time1h:50min2h:10min4.5d Maximum crack width1.13mm0.88mm0.59 mm 0.9kg/m 3 Initial crack time1h:25min1h:50min4d Maximum crack width1.34mm1.09mm0.81mm maximum crack width(24h) From the test results, for concrete with dosage for 1.5kg/m3, concrete crack first by dumbbell method which is superior to slab and ring method. dumbbell method need 2h:15min.Ring method need 6d; From view of the maximum crack width, it is 1.07mm by using dumbbell method which much larger than the other two methods. The concrete cracking performance can be reflected more obviously with larger Maximum crack width which make the crack be measured more easily and can reduce measurement error. concrete with dosage of 0.9kg/m3 and 1.2kg/m3 also shows the same trend.
Overall comparisons of the three test method dumbbellslabring dumbbellslabring sensitivitygoodabove averageaverage testing cycleshort long operabilitygoodaverageabove average application on job site goodabove averageaverage
Engineering Application Dumbbell method has been used to design concrete with high anti-crack performance for the second runway of Tianjin airport which is designed for test flight of the first Airbus A320 plane assembling in china. Testing photo with dumbbell method
airport runway construction (Tianjin, China) Concrete finishing
Runway (Tianjin, China)
Runway test for A320 （ China, May,2009 ）
A320 test successful （ China, May,2009 ）
Conclusion To sum up, from the view of sensitivity, test cycle, operability, application under airport construction, Dumbbell method is suitable for evaluating the early age concrete cracking performance with the following advantages: 1 、 stronger sensitivity 2 、 quickly testing 3 、 more accurate 4 、 easy measurement 5 、 convenient application under airport construction